O. Raquet1, E. Herms1, F. Vaillant2, T. Couvant21 Commissariat lEnergie Atomique (CEA), DEN/DPC/SCCME/LECA, 91191 Gif-sur-Yvette Cedex, France 2 Electricit de France (EDF), Les Renardires, R&D/MMC 77250 Moret sur Loing France
SCC OF COLD-WORKED AUSTENITIC STAINLESS STEELS IN PWR CONDITIONS
Keywords: stress corrosion cracking, cold work, austenitic stainless steels, hydrogen embrittlement, primary water
Susceptibility of sensitized austenitic stainless steels to Stress Corrosion Cracking (SCC) is a well known phenomenon identified in Boiling Water Reactor (BWR) oxidizing environments. Research associated with the case of BWR-type conditions have shown certain minimum levels of chloride and oxygen are required for SCC susceptibility [1 - 4]. The detrimental role of cold-work on the resistance of austenitic stainless steels to SCC was also clearly recognized in pure water BWR-type conditions in the presence of limited amounts of oxygen [5 - 9]. Cold-work was generally identified to increase Crack Growth Rates (CGR) and reduce the estimated crack initiation time for austenitic stainless steels tested in pure water containing oxygen at a temperature around 300C. The electrochemical potential usually measured for austenitic stainless steels exposed to hydrogenated Pressurized Water reactors (PWR) conditions appears well below the critical potential recognized for SCC initiation and too low to promote SCC susceptibility of these materials in absence of a significant amount of specific impurities. Consequently, solution annealed austenitic stainless steels, essentially of type AISI 304(L) and AISI 316(L), are generally considered as immune to SCC in hydrogenated primary water and these materials are thus widely used in PWRs. Some rather recent data [10, 11] have however demonstrated that austenitic stainless steels specimens that were severely cold-worked were susceptible to SCC in hydrogenated PWR environment under CERTs conditions. Failures of pressurisers heaters rods by SCC constructed from cold-worked austenitic stainless steels were additionally observed in several French power plants (12). The resistance of austenitic stainless steels to SCC in PWR conditions should be therefore re-evaluated with regard to the potential specific effects of cold-work. The objective of this paper is to detail the results obtained on SCC of cold-worked austenitic stainless steels. The main focus of this program
34 ADVANCES IN MATERIALS SCIENCE, Vol. 7, No. 1 (11), March 2007
is to assess SCC initiation susceptibility of steels considering the respective effects of cold-working mode and environmental parameters derived from standard PWR conditions.
Commercial purity AISI 304L plate material (30 mm in thickness) was the main material used for the study. The average grain size was 50 m. The level of ferrite (measured by Ferriscope) was between 5.5 % and 6.3 % in the middle of the plate and between 2% and 3% near the surfaces. Chemical composition of the 304L stainless steel used is given in Table I. Some tests were also performed on commercial AISI 316L stainless steels with the composition given in Table II. The samples were fully annealed at 1050C for 30 minutes under vacuum then quenched by argon in order to homogenize the austenitic phase and erase the prior cold work associated with sample manufacturing. After annealing the level of ferrite measured on test samples was approximately 3%. The annealing treatment was carried out before application of any cold-working procedure.
Table 1. Chemical composition 304L
304L C Cr Ni Mo Mn Si P S N W% 0.026 19.23 9.45 0.24 1.49 0.52 0.027 0.002 0.064
Table 2. Chemical composition 316L
316L C Cr Ni Mo Mn Si P S N W% 0.027 17.2 12.15 2.34 1.76 0.48 0.23 0.001 0.064
PWR test procedure
All of the tests performed in the framework of this study were carried out inside dedicated static 316L autoclaves including direct measurement of hydrogen partial pressure via the use of in-situ Ag/Pd probes. Hydrogen concentrations were in the range of 25 to 35 cc/kgH2O.STP in accordance with the usual PWR specification for primary water. Some specific tests were performed at low (1 cc/kgH2O.STP) or high (100 cc/kgH2O.STP) dissolved hydrogen concentrations. Pollutants (chloride, fluoride, sulfate) were measured after each test using ionic chromatography in order to verify that the concentration of each pollutant remained below the value of 50 ppb usually specified for PWR primary water. Examination of the fracture surface was performed using Scanning Electron Microscopy (SEM) in order to determine the morphology of fracture surface and the average depth of SCC. When mentioned, the average SCC growth rate was defined and calculated as follows: average SCC growth rate (m/hour) = maximum crack depth on fracture surface (m) / time to failure (hours).
O. Raquet, E. Herms, F. Vaillant, T. Couvant: SCC of cold-worked austenitic stainless steels 35
In order to analyze the effect of stress triaxiality on the susceptibility of the materials to SCC, some tests were performed on smooth specimens with a circumferential V-notch perpendicular to the tensile axis. The stress triaxiality coefficient induced by the notch was evaluated to be 1.55 (as per Bridgman formula). These specimens were fully annealed after machining the V-notch and thus no residual cold-work was initially present in material before testing in the water environment. The tensile/relaxation test was performed in nominal primary water conditions at 360C.
CERTs on specimens cold-worked by fatigue
The specimens cold-worked by fatigue were tested by CERT at 360C and 1x10-7s-1. All specimens were manufactured from AISI 304L of the composition mentioned above. These specimens were extracted from 8 mm diameter, 16 mm long samples previously cold-worked by fatigue at ambient temperature. The characteristics of the cyclic pre-loading procedure applied in the first stage of sample preparation were the following: tensile-compressive loading cycle, total strain 0,024 , extension rate 4x10-3s-1, 50 cycles. A small size tensile specimen was subsequently machined from inside the gage length of the initial fatigue sample. As a result of this procedure, the whole thickness of the 4 mm diameter tensile specimens extracted from the initial fatigue samples was cold-worked. The resulting surface hardness was 320HV (1.96N) and Ferriscope measurements indicated the formation of 6% of martensite phase from austenite in the cold-worked material. These specimens were then tested in CERTs at 360C at a constant extension rate of 1x10-7s-1. In order to obtain information on the role of martensitic phases formed during cold-working regarding the susceptibility of the material to SCC, some specimens were extracted from samples previously cold-worked by fatigue at 200C. At this temperature, the formation of martensite by cold-working is not anticipated. In this latter case, the initial surface hardness of the material was lower compared to specimens cold-worked at laboratory temperature: 255HV (1.96N) instead of 320HV (1.96N) due to the absence of martensitic transformation.
CERTs on specimens cold-worked by shot-peening
Shot-peening was selected to reproduce practical cases of superficial cold-working. The procedure for shot-peening provided a high initial surface hardness of 474HV (0.49N). The material hardness decreased with depth as shown in Figure 1 (profile of micro-hardness measurements). The cold-worked layer had a total depth of 250 m. The maximum residual stresses in surface of the material were in the range of 850 MPa (compressive). During a CERT test, the evolution of stress versus the applied strain was rather different inside the outer cold-worked layer compared to the stress variation evaluated in the bulk of the specimen. The increase in stress value was rapid for low values of strain in the cold-worked layer and during the majority of the CERT test duration; further evolution of stress inside the cold-worked layer was very slow after the first initially observed increase (see Figure 2). In order to study the specific effect of the initial surface hardness on material susceptibility to SCC, dedicated specimens were prepared from shot-peened samples to obtain progressively lower surface hardnesses. Electropolishing was
36 ADVANCES IN MATERIALS SCIENCE, Vol. 7, No. 1 (11), March 2007
used to eliminate a part of the outer hard cold-worked layer resulting from shot-peening and finally obtain test specimens with initial surface hardnesses of 300HV (0.49N) and 270HV (0.49N) respectively. All specimens were made from AISI 304L of the composition given earlier and were tested by CERT at 360C and 1x10-7s-1. With the aim to determine the effects of the dissolved hydrogen on the susceptibility of the material to SCC, some specimens that had been cold-worked by shot-peening (initial hardness 474HV) were tested by CERT in primary water of nominal composition at 320C with 3 different dissolved hydrogen levels: 1 cc H2/kgH2O.STP, 30 cc H2/kgH2O.STP and 100 cc H2/kgH2O.STP.
0 15 30 45
304L CW by shot peening
Fig. 1. profile of micro-hardness measurements onspecimen cold-worked by shot-peening
onstant load tests
These tests were performed on AISI 304arlier. The procedure for specimen cold-workingbjective of